Studies on Synthesis, Structural and Electrical Properties of
Complex Oxide Thin Films: Ba1-xSrxTiO3 and La2-xSrxNiO4
(Article begins on next page)
The Harvard community has made this article openly available.
how this access benefits you. Your story matters.
Podpirka, Adrian Alexander. 2012. Studies on Synthesis,
Structural and Electrical Properties of Complex Oxide Thin Films:
Ba1-xSrxTiO3 and La2-xSrxNiO4. Doctoral dissertation, Harvard
AccessedApril 17, 2018 3:40:50 PM EDT
This article was downloaded from Harvard University's DASH
repository, and is made available under the terms and conditions
applicable to Other Posted Material, as set forth at
© 2012 – Adrian A. Podpirka
Thesis Advisor Author
Professor Shriram Ramanathan Adrian A. Podpirka
Studies on Synthesis, Structural and Electrical Properties of
Complex Oxide Thin Films:
High performance miniaturized passives are of great importance for advanced nanoelectronic packages for several applications including efficient power delivery. Low cost thin film capacitors fabricated directly on package (and/or on-chip) are an attractive approach towards realizing such devices. This thesis aims to explore fundamental frequency dependent dielectric and insulating properties of thin film high-k dielectric constant in the perovskite and perovskite-related complex oxides. Throughout this thesis, we have successfully observed the role of structure, strain and oxygen stoichiometry on the dielectric properties of thin film complex oxides, allowing a greater understanding of processing conditions and polarization mechanisms.
In the first section of the thesis, we explore novel processing methods in the conventional ferroelectric, barium strontium titanate, Ba1-xSrxTiO3 (BST), using ultraviolet enhanced oxidation
techniques in order to achieve improvements in the dielectric properties. Using this method, we also explore the growth of BST on inexpensive non-noble metals such as Ni which presents technical challenges due to the ability to oxidize at high temperatures. We observe a significant
lowering of the dielectric loss while also lowering the process temperature which allows us to maintain an intimate interface between the dielectric layer and the metal electrode.
The second section of this thesis explores the novel dielectric material, Lanthanum Strontium Nickelate, La2-xSrxNiO4 (LSNO), which exhibits a colossal dielectric response. For
the first time, we report on the colossal dielectric properties of polycrystalline and epitaxial thin film LSNO. We observe a significant polarization dependence on the microstructure due to the grain/grain boundary interaction with charged carriers. We next grew epitaxial films on various insulating oxide substrates in order to decouple the grain boundary interaction. Here we observed substrate dependent dielectric properties associated with induced strain. We also observe, due to the p-type carriers in LSNO, pn junction formation when grown epitaxially on the conducting oxide degenerate n-type Nb-doped SrTiO3. Finally we explore the growth
mechanism of epitaxial LSNO as a function of high oxygen content. Due to the ability for LSNO to take in interstitial oxygen, a reoriented growth is observed at a critical thickness, thereby allowing us to vary anisotropy as a function of deposition conditions.
Table of Contents
Title ... i
Abstract ... iii
Table of Contents ... v
Table of Figures ... x
Published Work ... xxi
Acknowledgments ... xxiii
Dedication ... xxviii
Introduction... 11.1 Complex Oxides ... 1 1.2 Dielectric Materials ... 7 1.2.1 Ferroelectrics ... 10
1.2.2 Colossal Dielectric Constant Materials ... 12
184.108.40.206 Mechanism for Colossal Dielectric Response ... 14
220.127.116.11 Hopping Charge Transport ... 14
18.104.22.168 Interfaces ... 15
1.3 Motivation of Thesis ... 19
1.3.1 Bypass Capacitors for Next Generation System on Package Technology ... 19
1.3.2 Material Studied ... 23
22.214.171.124 BST... 23
Outline of Thesis ...29
Experimental Methods ...31
3.1 Thin Film Deposition and Processing ... 31
3.1.1 Sputtering... 31
126.96.36.199 DC Sputtering ... 32
188.8.131.52 RF Sputtering ... 32
184.108.40.206 Magnetron Sputter Deposition ... 33
3.1.2 Electron beam deposition (E-beam) ... 34
3.1.3 Processing Parameters and Post-processing techniques ... 35
220.127.116.11 Room Temperature Growth ... 35
18.104.22.168 Epitaxial Growth of oxide thin films ... 39
3.2 Ultraviolet Photon Film Synthesis ... 40
3.2.1 Photochemistry of Oxygen ... 40
3.2.2 Recent Review of UV enhanced oxidation ... 41
3.3 X-Ray Characterization ... 42
3.3.1 Fundamentals of Diffraction ... 42
3.3.2 X-Ray Diffraction (XRD) ... 45
3.3.3 Glancing Incidence X-Ray Diffraction (GIXRD) ... 46
3.3.4 X-Ray Reflectivity (XRR) ... 47
3.3.5 Azimuthal Scan (ϕ Scan) ... 49
3.3.6 Rocking Curve ... 50
3.3.7 Reciprocal Space Map (RSM) ... 51
vii 22.214.171.124.1 Strain ... 54 126.96.36.199.2 Mosaicitiy ... 56 3.3.8 Pole Figures ... 57 3.4 Electrical Measurements ... 59 3.4.1 Electrical Contacts ... 59
3.4.2 Metal-Insulator-Metal Devices and Interdigitated Capacitor Devices ... 60
3.4.3 Impedance Spectroscopy ... 62
3.4.4 Metal-Semiconductor and pn Junctions ... 64
3.5 Transmission Electron Microscopy (TEM) ... 65
4.1 Photon Assisted Oxidation in BST ... 67
4.1.1 Abstract ... 67
4.1.2 Introduction ... 67
4.1.3 Experimental ... 68
4.1.4 Results ... 69
4.1.5 Conclusion ... 77
4.2 Novel Processing Route for BST on Non-noble metal substrates ... 78
4.2.1 Abstract ... 78 4.2.2 Introduction ... 78 4.2.3 Experimental ... 80 4.2.4 Results ... 82 4.2.5 Conclusion ... 98
5.1 Colossal Dielectric Response in Polycrystalline Thin Film LSNO ... 99
5.1.1 Abstract ... 99
5.1.2 Introduction ... 99
5.1.3 Experimental ... 100
5.1.4 Results ... 101
5.1.5 Conclusion ... 122
5.2 pn Junction Behavior in Epitaxial LSNO on Nb:SrTiO3 ... 123
5.2.1 Abstract ... 123
5.2.2 Introduction ... 123
5.2.3 Experimental ... 124
5.2.4 Results ... 125
5.2.5 Conclusion ... 149
5.3 Role of Strain in Thin Film LSNO ... 149
5.3.1 Abstract ... 149
5.3.2 Introduction ... 150
5.3.3 Experimental ... 151
5.3.4 Results ... 152
5.3.5 Conclusion ... 163
5.4 Growth and Reorientation in Epitaxial LSNO on SrTiO3 ... 164
5.4.1 Abstract ... 164
5.4.2 Introduction ... 164
5.4.3 Experimental ... 166
5.4.5 Conclusion ... 189
Table of Figures
Figure 1: Periodic Table of Elements. Transition metals are shaded in purple. Reprinted with permission from Ref.. Copyright 2011, Model Science Software Inc. ... 2
Figure 2: The perovskite ABO3 structure is given in the center (A site – green, B site – blue, O
site – red). Due to the interplay of competing energies, properties can be varied significantly with small variation in doping and strain. Reprinted with permission from Ref. . Copyright 2011, Annual Reviews. ... 4
Figure 3: K2NiF4 structure (Tetragonal; I4/mmm). Fluorine site is red, Nickel site is grey and
Potassium site is green. Created with Ref.. ... 5
Figure 4: General view of the polarization mechanisms as a function of frequency showing approximate mechanism as to where polarization takes place. Reprinted with permission from Ref.. Copyright 2003, American Institute of Physics. ... 8
Figure 5: Dielectric constant as a function of temperature for a BaTiO3 crystal. Reprinted from
Ref.. Copyright 1949 by the American Physical Society. ... 12
Figure 6: Behavior of CCTO single crystal showing typical colossal dielectric properties. Reprinted with permission from Ref. . Copyright 2008, American Institute of Physics. ... 13
Figure 7: Maxwell-Wagner two layer capacitor model. Adapted from Dielectrics and Waves (Ref.). ... 18
Figure 8: Moore's Law and System Integration Law. Reprinted with permission from Ref. .Copyright 2006, IEEE. ... 20
Figure 9: Projected evolution from Surface Mount Technology (SMT) to Embedded Passives. Reprinted with permission from Ref.. ... 21
Figure 10: Future view of a System-on-Package. Note the placement of the decoupling capacitor. Reprinted with permission from Ref.. Copyright 2006, IEEE. ... 22
Figure 11: Effect of cation ratio on the crystal structure of BST. Reprinted with permission from Ref. . Copyright 1997, American Institute of Physics. ... 24
Figure 12: Effect of cation ratio on the Curie temperature of BST. Reprinted with permission from Ref.. Copyright 1997, American Institute of Physics. ... 25
Figure 13: Electrical conductivity in polycrystalline BaTiO3 as a function of partial pressure.
Reprinted with permission from Ref.. Copyright 1985, Annual Reviews. .... 26 Figure 14: Schematic drawing of the sputtering process. ... 32 Figure 15: Schematic diagram of e-beam deposition. ... 34
Figure 16: Structural evolution in polycrystalline films as a function of substrate temperature and argon gas sputtering pressure. Reprinted with permission from Ref. . Copyright 1977, Annual Reviews. ... 36
Figure 17: pO2 vs temperature diagram showing processing window in which oxides of Ba, Sr
and Ti are stable with metallic Ni as derived from elligham diagrams. Reprinted with permission from Ref.. Copyright 2008, American Institute of Physics. ... 38
Figure 18: Load lock UV annealing setup that were used in these experiments. ... 41
Figure 19: (a) Bragg’s Law and the (b) relationship of the incident, diffracted and scattering vectors with respect to the crystal. Plants of atoms are indicated by dotted lines. Reprinted with permission from Ref.. Copyright 2009, IOP Publishing LTD.45
Figure 20: Measurement geometry of a glancing incidence x-ray diffraction scan. Note the random orientation of the grains allowing for the satisfaction of Bragg's law. Striped lines indicate lattice planes. ... 47
Figure 21: x-ray reflectivity diagram. ... 49 Figure 22: Typical ø scan observed showing four- fold symmetry. ... 50
Figure 23: (A) Schematic drawing of ray diagram showing a rocking curve. (B) Rocking curve for a single crystal sample. Note the lattice planes that are all contributing to the diffraction at precisely the same moment. (C) Rocking curve for a mosaic or textured sample. Note the lattice plane mosaicity contributing to the broadening. ... 51
Figure 24: Reciprocal Space Map showing the Ewald sphere construction. Reprinted with permission from Ref.. Copyright 2009, IOP Publishing LTD. ... 53
Figure 25: RSM data for a (a) strained and (b) partially relaxed film. Reprinted with permission from Ref.. Copyright 2009, IOP Publishing LTD. ... 54
Figure 26: Reciprocal Space Maps showing the effects of relaxation, strain and misorientation. Reprinted with permission from Ref.. Copyright 2010, Rigaku Corporation. 55
Figure 27: Schematic diagram showing the degree of relaxation in epitaxial films. Reprinted with permission from Ref.. Copyright 1997, American Institute of Physics. ... 56
Figure 28: Spreading of the reciprocal space map as a function of mosaicity. Reprinted from Ref.. ... 57
Figure 29: Setup for GADDS scan. Reprinted with permission from Ref.. Copyright 2000, JCPDS-International Centre for Diffraction Data. ... 58
Figure 30: (a) diffraction poles from a single crystal (b) diffraction cones from a polycrystalline material. Reprinted with permission from Ref.. Copyright 2000, JCPDS-International Centre for Diffraction Data. ... 59 Figure 31: (A) Cross section view of MIM structure. (B) Top view of MIM structure. .. 61 Figure 32: Schematic image of an IDC structure... 62
Figure 33: GIXRD patterns of BST thin films annealed at 700°C for 60 minutes (a) with UV treatment and (b) without UV treatment. Dotted lines represent the BST (60/40) bulk peak position (JCPDF #00-034-0411). ... 71
Figure 34: Change in lattice parameter as a function of annealing temperature for BST films annealed with (red filled circles) and without (black filled squares) UV-assist. .. 72
Figure 35: The variation in (a) FWHM and (b) lattice parameter of the 700°C annealed UV-assist (red filled circles) and non-UV treated (black filled squares) BST (60/40) films as a function of annealing time. ... 73
Figure 36: Dielectric response as a function of applied bias for the BST films annealed at 700oC with (red filled circles) and without UV-assist (black filled squares). ... 76
Figure 37: Variation of leakage current density with applied reverse bias for the BST thin films annealed at 700oC with (red filled circles) and without UV-assist (black filled squares). ... 77 Figure 38: Flow Chart of preparation of BST films for electrical characterization ... 81
Figure 39: x-ray diffraction pattern of BST grown on nickelized sapphire annealed in reduced conditions (A) and air (B). Annealing temperatures are displayed on graph. All samples measured at room temperature. Solid vertical lines – Nickel (JCPDS# 01-071-3740),
Dotted lines – Nickel Oxide (JCPDS# 00-004-0835), Dashed vertical line – BST (taken for BST(77/23) – JCPDS# 00-044-0093). ... 83
Figure 40: Cross sectional TEM micrograph of 150 nm thick BST film deposited on nickelized Si (100) substrate, annealed at 973K under reducing atmosphere. (A) Selected area diffraction pattern recorded from the Ni-BST interface. (B) Corresponding dark field image recorded using the (110) reflection of BST. (C) High-resolution image of Ni/BST interface... 84
Figure 41: Capacitance density and dielectric loss tangent for 150nm thick BST thin film grown on Ni bottom electrode with Pt top contacts. Films were treated under reducing anneal at 973K (black squares) and reoxidized conventionally (red circles) or with UV-enhanced oxidation (blue triangles) at 573K. Dielectric constant equivalents of capacitance density are given by the dashed blue line and labeled accordingly. ... 86
Figure 42: AC conductivity as a function of applied electric field measured at 1 Mhz for varying thickness BST samples annealed at 973K under reducing conditions. Samples prepared on nickelized silicon. ... 88
Figure 43: Cross sectional TEM micrograph of BST film grown on nickelized Si substrate, re-oxidized at 573K under UV irradiation. (A) Selected area diffraction pattern recorded from the Ni-BST interface. (B) The corresponding dark field image recorded using the (110) reflection of BST. (C) The high resolution image of Ni/BST interface revealing no additional reaction layers. ... 92
Figure 44: Capacitance density and dielectric loss tangents of reduced 150nm BST films reoxidized at 373K (A) and 473K (B) with UV and conventionally (without UV). Samples are grown with Ni bottom electrode with top Pt contact. ... 94
Figure 45: Capacitance density and dielectric loss tangent for 150nm thick BST thin film grown on Pt bottom electrode with Pt top contacts. Dielectric constant equivalents of capacitance density are given by the dashed blue line and labeled accordingly. . 96
Figure 46: Leakage current density as a function of electric field for 150nm thick BST grown on Ni bottom electrode with top Pt electrode. ... 97
Figure 47: Leakage current density as a function of electric field for 150nm thick BST with Pt top and bottom electrodes ... 98
Figure 48: x-ray diffraction taken from a LSNO thin film. Vertical red dashed lines indicate La2NiO4 JCPDS data (file # 00-011-0557) with diffraction planes indicated above.
Figure 49: Plane view SEM image of LSNO surface after annealing. Grain size is approximately 150 nm. ... 103
Figure 50: Dielectric constant of LSNO thin film (black squares) from this work and single crystal data (blue squares) taken at 300K from Krohns et al. is shown for comparison. Inset is an impedance spectra from the LSNO film. Model fitting to data is plotted in red. ... 105
Figure 51: Dielectric response of LSNO thin films as a (A) function of frequency and (B) temperature for two representative frequencies. (C) Loss tangent as a function of frequency for various temperatures. ... 106
Figure 52: (A) Conductivity vs. frequency as a function of temperature. (B) Power law exponent, n, as a function of temperature. Inset shows representative fitting curve.108
Figure 53: Dielectric permittivity as a function of frequency for Pt, Pd and Ag contacted LSNO thin films. The bottom contact is Pt in all cases synthesized identically. Metal work functions are labeled on the graph. ... 112
Figure 54: Conductivity as a function of frequency for (A) Ag and (B) Pd contact thin films at different temperatures. ... 113
Figure 55: (A) Arrhenius relationship showing the DC activation energy for the Ag and Pd electroded films. (B) Power law exponent, n, for Ag and Pd contacted LSNO as a function of temperature. ... 114
Figure 56: (A) Impedance spectra of Pt contacted LSNO thin films as a function of bias. (B) Real permittivity as a function of frequency derived from the impedance plot for different applied biases. ... 116
Figure 57: (A) Impedance spectra of Pd contacted LSNO thin films as a function of bias. (B) Real permittivity as a function of frequency derived from the impedance plot for different applied biases. ... 117
Figure 58: (A) Impedance spectra of Ag contacted LSNO thin films as a function of bias. (B) Real permittivity as a function of frequency derived from the impedance plot for different applied biases. ... 118
Figure 59: (Top) Dielectric constants and (Bottom) tunability of Pt, Pd and Ag contacted LSNO as a function of applied bias at (column A) 100 Hz, (column B) 1kHz, and (column C) 10 kHz. ... 120
Figure 60: Dielectric constant of sample prepared without and with post processing UV annealing treatment. Inset: Impedance spectra of two previously compared samples. ... 122
Figure 61: Diffraction pattern taken from epitaxial LSNO film of 110nm thickness on 0.7% Nb:STO substrate. (00l) family of peaks are present. ... 127
Figure 62: Epitaxial relation for 110nm thick LSNO on 0.7% Nb:STO of the (114), (103), (101) and (204) planes. (111) Nb:STO plane scanned for reference. Peaks indicate 4-fold symmetry as expected for LSNO films. ... 128
Figure 63: Linear plots of current density as a function of voltage for (A) Nb0.7%-110 nm, (B) Nb0.7%-220 nm and (C) Nb0.1%-110 nm samples. Log linear current density plot in the positive bias of (D) Nb0.7%-110 nm, (E) Nb0.7%-220 nm and (F) Nb0.1%-110 nm samples. ... 130
Figure 64: Ideality of the junction as derived from Figure 63 for (black squares) Nb0.7% - 110nm, (red circles) Nb0.7% - 220nm and (blue triangles) Nb0.1% - 110nm. .. 132
Figure 65: (A) Log-linear current density comparison of 110nm (black squares) and 220nm (red circles) samples grown on 0.7% Nb:STO. (B) Log-linear current density comparison of 110nm thick LSNO grown on 0.1% Nb:STO (blue triangles) and 0.7% Nb:STO (black squares). Inset shows linear comparison. ... 134
Figure 66: Capacitance-voltage curves for Nb0.7%-110 nm at (A) 1 kHz and (B) 10 kHz, for Nb0.7%-220 nm at (C) 1 kHz and (D) 10 kHz, and for Nb0.1%-110 nm at (E) 1 kHz and (F) 10 kHz. ... 137
Figure 67: C-2-V curves for Nb0.7%-110nm at (A) 1 kHz and (B) 10 kHz, for Nb0.7%-220nm at
(C) 1 kHz and (D) 10 kHz, and for Nb0.1%-110nm at (E) 1 kHz and (F) 10 kHz as derived from Figure 66. ... 139
Figure 68: Built-in voltage measured at (A) 1 kHz and (B) 10 kHz plotted as a function of temperature for Nb0.7%-110 nm (black squares), Nb0.7%-220 nm (red circles) and Nb0.1%-110 nm (blue triangles)... 141
Figure 69: Dielectric loss tangent for 110nm at (A) 1 kHz and (B) 10 kHz, for Nb0.7%-220 nm at (C) 1 kHz and (D) 10 kHz, and for Nb0.1%-110nm at (E) 1 kHz and (F) 10 kHz as a function of temperature. ... 142
Figure 70: (Top row) Capacitance density as a function of frequency plotted at different temperatures for (A) Nb0.7%-110nm, (B) Nb0.7%-220 nm, and (C) Nb0.1%-110 nm. (Bottom row) Capacitance density as a function of applied negative bias for (D) Nb0.7%-110 nm, (E) Nb0.7%-220 nm, and (F) Nb0.1%-Nb0.7%-110 nm. ... 144 Figure 71: (G/ω) vs. frequency of (A) Nb0.7%-110 nm, (B) Nb0.7%-220 nm and (C)
Nb0.1%-110 nm films measured at 0V bias as a function of temperature. Inset in Figure 71b shows the resonance frequency peak positions for the Nb0.7%-220 nm sample.146
Figure 72: Built-in voltage as a function of frequency for (A) Nb0.7%-110 nm, (B) Nb0.7%-220 nm, and (C) Nb0.1%-110 nm as derived from Figure 70. ... 147
Figure 73: θ-2θ scans for LSNO films on (A) STO, (B) LAO and (C) SLA substrates. Phi scans from symmetric peaks for LSNO grown on (D) STO, (E) LAO and (F) SLA. Substrate ϕ scans are plotted as a reference. ... 153
Figure 74: Reciprocal space maps of LSNO films grown on (A) STO, (B) LAO and (C) SLA substrate. LSNO on STO is shown to be grown under tensile strain whereas LSNO on LAO and SLA are under compressive strain. Dashed vertical line is used to visualize coherent growth i.e. same in-plane qx value. ... 155
Figure 75: (A) Diffraction pattern of LSNO film grown on ALO. * indicated reflections from substrate holder. (B) Pole figure of the (200) LSNO reflection. (C) Pole figure take at 44° showing reflections from both the (113) sapphire (six-fold symmetry) and the (114) LSNO. χ is the radial direction and ϕ is the angular coordinate. ... 158
Figure 76: (A) Comparison between two methods used for analysis of dielectric response of LSNO on LAO substrate. Inset shows closeup of the IDC structure. (B) Dielectric constant as a function of frequency for LSNO on LAO, STO, SLA and ALO substrates taken at 303K ... 160
Figure 77: Dielectric constant as a function of temperature for LSNO on (A) LAO, (B) SLA, (C) STO and (D) ALO. Insets show the loss tangent as a function of temperature. . 162
Figure 78: Diffraction pattern of LSNO on STO as a function of thickness showing the formation of the (200) phase... 168
Figure 79: x-ray reflectivity of 25nm thick LSNO on STO. Inset (A) Phi scan showing of 25nm thick (103) LSNO on STO. Inset (B) Rocking curve data for 25nm thick LSNO (006). ... 169
Figure 80: Crystal structure of LSNO. (100) and (001) planes are shown in gray and blue, respectively. Created with Ref.. ... 170
Figure 81: Rocking curve data as a function of thickness for the (200) LSNO peak. Broadness of 50nm LSNO indicates weak texturing. Offset of peak position is due to alignment of substrate. ... 171
Figure 82: TEM-Bright field image shows the of LSNO film of 100 nm thickness on STO substrate. SAED pattern from LSNO film and STO substrate are shown as insets.173
Figure 83: TEM lattice image of LSNO on STO shows the orientation evolution of LSNO film grown on STO. FFT patterns (A-E) show the changes in the orientation of LSNO film across the critical thickness of 15 nm. ... 174
Figure 84: HRTEM image reveals the existence of critical thickness favoring LSNO //STO -OR1 and LSNO//STO-OR2 at low and high thicknesses respectively. The corresponding FFT patterns obtained from different layers are shown as insets. ... 175
Figure 85: TEM (A) bright field image and (B) lattice image recorded from LSNO film showing dense columnar microstruture of OR-2 region. Columnar structure is marked using arrow marks and lines in bright field and lattice image respectively. ... 176
Figure 86: EELS spectra collected from STO substrate (A-C) and LSNO film (D-F) regions are shown with their characteristic energy loss edges and energy loss near edge structures (ELNES) that confirm the formation of phase pure LSNO film on STO. ... 178
Figure 87: Pole figure for the (105), (006) reflection of thin film LSNO at 25nm, 50nm 100nm and 150nm. Simulation pole figure for the (105),(006) reflection with (001) orientation and (100) orientation. ... 180
Figure 88: Pole figure for the (114) reflection of thin film LSNO at 25nm, 50nm 100nm and 150nm. Simulation pole figure for the (114) reflection with (001) orientation and (100) orientation. ... 182
Figure 89: Dielectric properties of LSNO thin film of (A) 25nm and 50nm and (B) 75nm, 125, and 150nm grown on STO. ... 184
Figure 90: Dielectric loss tangent for LSNO thin film of (A) 25nm and 50nm and (B) 75nm, 125, and 150nm grown on STO. ... 186
A. Podpirka, B. Viswanath, and S. Ramanathan. Heteroepitaxy of La1.875Sr0.125NiO4 thin
films on SrTiO3: orientation evolution and dielectric (under review).
A. Podpirka, A. Tselev and S. Ramanathan. Synthesis and frequency-dependent
dielectric properties of epitaxial La1.875Sr0.125NiO4 thin films. (under review).
S. D. Ha, M. Otaki, R. Jaramillo, A. Podpirka and S. Ramanathan. Stable metal-insulator transition in epitaxial SmNiO3 thin films, Journal of Solid State Chemistry, in press, 2012
A. Podpirka and S. Ramanathan. Heteroepitaxial La2-xSrxNiO4-Nb-doped SrTiO3
Junctions: Synthesis and Rectification Characteristics. J. Electrochemical Society 159, H72 (2012).
M.W. Cole, R.C. Toonen, S.G. Hirsch, M. Ivill, E. Ngo, C. Hubbard, S.Ramanathan and
A. Podpirka. An elegant post-growth process science protocol to improve the material
properties of complex oxide thin films for tunable deivce applications. Integrated
Ferroelectrics 126 34 (2011).
A. Podpirka, and S. Ramanathan. Thin film colossal dielectric constant oxide La 2-xSrxNiO4: Synthesis, dielectric relaxation measurement and electrode effects. Journal of Applied Physics 109, 014106 (2011).
A. Podpirka, K.B. Viswanath and S. Ramanathan. Active low temperature oxidation as
a route to minimize electrode-oxide interface reactions in nanoscale capacitors. Journal of Applied Physics. Journal of Applied Physics. 108, 024106 (2010).
M.W. Cole, E. Ngo, A. Podpirka, S. Ramanathan, M. Ivill, R.C. Toonen, S.G. Hirsch, and C. Hubbard. Improved material properties of complex oxide thin films for applications in phased array antennas. Earth and Space 2010: Engineering, Science,
Construction and Operations in Challenging Environments 3444 (2010).
A. Podpirka, and S. Ramanathan. Tranference numbers for in-plane carrier conduction
in thin film nanostructured Gadolinia-Doped Ceria under varying oxygen partial pressure.
Journal of American Ceramic Society 92 2400 (2009).
M. W. Cole, A. Podpirka, and S. Ramanathan. A post-growth processing methodology to achieve barium strontium titanate thin films with low dielectric loss and high tenability for reconfigurable tunable devices. Journal of Material Science 44, 5332 (2009).
A. Podpirka, M.W. Cole, and S. Ramanathan. Effect of photon irradiation on structural,
dielectric and insulating properties of Ba0.60Sr0.40TiO3 (BST) thin films. Applied Physics Letters 92, 212906 (2008).
The Ph.D. is a long and arduous journey, requiring sacrifice and commitment. Completing it is more than the product of one’s work; it is also a testament to the people who supported the endeavor. Without those people, this degree is impossible—and to them I am tremendously grateful. So now comes the difficult part of actually putting that gratitude into words. I’ve frequently thought about how this acknowledgment will sound. It definitely seems easier than it is. Now it is my turn.
I would like to first acknowledge my advisor, Prof. Shriram Ramanathan, for guiding me through my entire degree. He was always available to discuss the project, challenge me by questioning my work, provide feedback, and give me the resources to do the necessary experiments. He was always passionate about the project which rubbed off on me and gave the freedom to work at my own pace (as long as I had results and a paper ready!). He gave me the freedom when I needed it and hustled me along when I was lagging. I could not have asked for a better advisor.
I would also like to thank my thesis committee, Prof. Frans Spaepen and Prof. Roy Gordon, who made the qualifier and defense process painless and gave interesting suggestions, great feedback, and thought-provoking questions. More importantly, they were available throughout my graduate school career, both for guidance and for helpful discussions.
I am greatly indebted to my funding sources that allowed me to work on these projects; I am very lucky those sources fit so well with my interests. My first project was sponsored by the Army Research Lab under the direction of Dr. Melanie Cole. Thinking about the application of my work to real-world problems greatly influenced my experiments and allowed me to make
relevant advances. In the past 3 years, my project has also been supported by a Semiconductor Research Corporation (SRC) grant. I would like to thank our industry liaisons, Dr. Larry Mosley and Dr. Rajasekaran Swaminathan from Intel that gave helpful feedback in our monthly meetings.
The Center for Nanoscale Systems (CNS) staff at Harvard has been extremely helpful with running all the experiments necessary for lithography, deposition, and characterization. In particular, I would like to thank Greg Lin for help on XPS, Steve Hickman for photolithography, and Jason Tresback for the low temperature probe station.
I am grateful for all the mentoring I have received in x-ray diffraction throughout my time at Harvard. Scott Speakman at MIT has been a tremendous part of this work, especially pertaining to the epitaxial and textured films. He was always available to discuss the experiments, help with alignment, and otherwise assist me. Anyone who has ever worked with x-rays knows just how important this is!
Of course, I wouldn’t even be here without the prior foundation I received in my undergraduate training. I would like to acknowledge the material science department at Columbia University for providing the background necessary. In particular, I would like to thank Prof. Baily, Prof. Siu-Wai Chan, Prof. O’brien, Prof. Labowitz and Prof. Guha who shaped my understanding of the field. Working with Prof. Chan and Prof. Laibowitz and taking the classes of Prof. Guha and Prof. Baily definitely steered me towards thin film oxide electronics.
Any degree that takes this long requires some sense of normalcy. Throughout my youth, I have grown up being a part of the Ukrainian scouting organization, PLAST. From my first year in Boston, I have worked as a scout counselor with a troop. Although often time-consuming, being a scout counselor was a great way to complement my studies. Working with
youth and acting as a mentor has allowed me to better know myself. The group of friends that I know from scouting and my scout fraternity Лісові Чорти has helped me through the years. The camps I have run and the friends I have made have allowed me to keep the continuity from my youth that is such an intricate part of my life. The Ukrainian community in Boston has been a big part of this continuity, as has the Ukrainian club at Harvard. Having weekly pierogies after church on Sunday and celebrating the holidays with the community gave that sense of home that gives the sanity check needed to complete each week!
Similarly, hockey at Harvard, with Dudley House and the summer league has been an outlet for all my frustrating experiments. A special thanks to Mark who passed the list on to me. A shout out to all the regulars who were at the weekly skate with me: Dave, Pardo, Rod, Philip, Dan, Alex, Tim, Jon, Dustin, Orest and Jesse. Having free ice at Harvard definitely tacked on a few years to this Ph.D!
The beauty of going to school at Harvard is to be surrounded by the best and the brightest. Students and postdocs at Harvard have given me great discussions, terrific collaboration, and a great all-around experience. We struggled through classes together and together stressed over our qualifiers. So I would like to thank my lab and office mates with whom I have had the pleasure to work these past few years. Although I have crossed paths with many through these years, I especially wanted to single out Karthik, Dima, Bo, Masaru, Ko, Charbel, Dan, Jason, Gulgun, You, Viswanath, Brian, Alex and Gokul. Also, I want to thank Don at Rowland for all the machining these past few years.
We are defined by the people we hold as our friends and I have been blessed by a number who have been with me through all the high points and the low points of my graduate school career. It is those who stick by in thick and thin that are true friends. To Aleks and Molly for
putting me up every visit and listening to me complain so much, to Subtelny who has worked so hard alongside me with scouts every weekend, to Rositsa for the excellent help with x-ray diffraction, to Rob, Russel and Frank who were there for me whenever I came to New York and needed that beer in the tough times, to Aaron, Eric, Jess, Libby and the rest of the rowers who have been an extended family to me, to Hiten for always letting me crash in London and showing me what jingoistic British patriotism was, to Gorana for being the best roommate, Bro (Article 22 of the Bro code), and wingwoman that anyone could ask for and traveling the world with me, to Maria for educating me that Sweden is the greatest country in the world, to Vanessa for not murdering me as a roommate, to Bill for his passionate sports debates and to Taylor for the political debates that have made this office an interesting as well as awkward place! There have been countless more that I could not possibly fit into this acknowledgement. Thank you all!
In graduate school some of my closest friends became the coworkers who sat with me day in and day out – Kian, Raf and Sieu. Our annual pilgrimage to Hells night has definitely been a highlight of culinary disaster! Working alongside them has been a great experience and I can only wish that my coworkers in the coming years can be like them. In particular, Kian has been a true Bro and a great roommate these past few years.
My best friends have been with me every step of the way; Pavlo, Xrysta, Tanya and Chris, Petro and Duzyj and Anya. Really, I really can’t thank you enough for being there through it all, traveling with me, partying with me and just being there for me. Graduate school is a huge commitment but through it all, true friends are a constant. I couldn’t have asked for a better bunch of friends.
Finally, yet most importantly, I want to thank my family. They have been so supportive of this degree. My brothers, Roman and Victor, gave me so much; visiting me randomly, laughing
and fighting with me, dealing with the me through my frustration and sending me anything I have forgotten from home. You both have definitely shaped my world! My father, who throughout my entire life stressed the importance of education and provided me with everything I needed to obtain it. You have given me everything I could have ever imagined. I can only hope I have made you proud. Most importantly, I want to thank my mother, to whom I dedicate this thesis. She sat with me through homework, never gave up on me, took me to speech therapy classes when I struggled in school, worked with me through all those college apps, drove me to all the practices and lessons, even came to take care of me in grad school when I was sick. She supported me in all of my endeavors. This degree is a reflection of all the hard work and sacrifices my parents put into raising me. I really cannot have asked for a more supportive and close-knit family.
This thesis is dedicated to my mother, Roxolana Podpirka, who always believed in me and my work and never let me give up. Though she didn’t see this day, she was with me every step of the way. I miss you more than words can describe.
After my first publication Adio,
It’s fascinating.. if only I knew what it said. Congratulations! Its not everbody that can say what most people don’t understand …and in so many words. I’m really proud of you. And we can discuss your paper next time I see you because of course I am going to read it.
1.1 Complex Oxides
The three transition series form the short group of elements in the periodic table, interposed between the longer main groups, highlighted in Figure 1. The occurrence of these elements as well as the varied properties of their compounds is a feature of the progressive filling of d orbitals across the series. These transition metal elements readily form oxides. The functionality of such compounds when considering monoxide MOx where M is the transition
metal is quite significant even with the simplest compounds. Transition metal oxides range from good insulators (HfO2) which is now replacing SiO2 in gate dielectrics to Metals (RuO2).1,2
Transition metal compounds show transitions from a metallic to a non-metallic state as a function of temperature and strain (VO2) however, as complexity of the oxides increases, so does
Figure 1: Periodic Table of Elements. Transition metals are shaded in purple. Reprinted with permission from Ref.. Copyright 2011, Model Science Software Inc.
The more complex ternary and higher-order oxides possess even more exotic properties such as ferroelectrics, colossal magnetic resistance, colossal dielectric constants and high temperature superconductivity.6,7,8,9 One family of transition metal oxides that has received a disproportionate amount of attention consists of compounds with the chemical formula ABO3
that crystallize into the perovskite structure, shown in the center of Figure 2. The A and B sites can support metal cations with a wide range of size and valence giving rise to a large diversity of physical phenomena as shown in Figure 2. No other material group has shown such varied characteristic by the doping of different cations while maintaining the same crystal structure. Control over the positional ordering of the cations provides an additional tool for mediating the electronic response when the A or B site contain mixtures of two (or more) different atoms.
Perovskites can be descried in terms of close packing of AO3 layers where the B site
cations occupy all of the resultant BO6 oxygen octahedral. When the AO3 layers are arranged in
cubic close packing, the BO6 octahedra are connected through corner sharing and the structure is
termed a cubic perovskite. In an ideal cubic perovskite the A and B cations realize their equilibrium bond distances to oxygen without inducing any distortion of the unit cell and
) ( 2 B O
d − = − . This leads to cubic symmetry and a resulting Goldschmidt tolerance factor of 1 where t=r(A+rO)/ 2(rB +rO).10 The cation radius may vary significantly which plays an important role in the crystal structure and in turn, the final electronic properties of the material. Interestingly, when dealing with thin films, these properties can be induced through epitaxial growth and strain engineering.
Figure 2: The perovskite ABO3 structure is given in the center (A site – green, B site –
blue, O site – red). Due to the interplay of competing energies, properties can be varied significantly with small variation in doping and strain. Reprinted with permission from Ref. . Copyright 2011, Annual Reviews.
Related to the perovskites, and built upon its initial structure is the layered Ruddlesden-Popper phase. Ruddlesden-popper structure is a perovskite structure with a rocksalt layer on either end as shown in Figure 3. The structure is known commonly as the K2NiF4. In the past 20
years, the key stimulus to study the K2NiF4 structure has arisen from the high-Tc superconductors
La2CuO4. 12 Due to similarity in the crystal structure, nickelates are being investigates to better
understand the origins of superconductivity in layered perovskites. However, layered nickelates also contain rich physics from large intercalation of oxygen into the lattice, to charge ordering and high ionic conductivity which will be discussed in more detail is chapter 188.8.131.52
Figure 3: K2NiF4 structure (Tetragonal; I4/mmm). Fluorine site is red, Nickel site is grey
and Potassium site is green. Created with Ref..
Among complex oxides, the ABO3 and related layered compounds stand out for their
unique properties. The subtle interplay between competing energy scales in complex oxides results in a variety of orderings of the spin, charge and orbital degrees of freedom. Charge
transport can exhibit colossal magnetoresistance, metal-to-insulator transitions or insulator-to-superconductor transitions in strongly correlated compounds. Cooperative alignment of electric dipoles or spins leads to ferroelectricity or ferromagnetism, respectively. Tilting and buckling of oxygen octahedral, which results from antiferrodistortive structural ordering can couple to other modes in the system, driving structural and electronic phase transitions. All these transformations can be seen in Figure 2.11 With the wealth of functional properties, complex transition metal oxides are rich picking ground for physicists, engineers and material scientists alike.
In this thesis, the properties of two complex oxides in thin film form will be discussed: Ba1-xSrxTiO3 (BST) and La2-xSrxNiO4 (LSNO), pertaining mostly to their dielectric properties.
The first part of the thesis delves into the solid solution of BaTiO3 and SrTiO3 with the chemical
structure Ba1-xSrxTiO3 (BST) which displays large paraelectric polarization. In this material we
investigate the effect of oxygen stoichiometry on the dielectric properties and investigate novel processing methods for growth on non-noble electrodes. The second material studied is of the ruddlesden-popper phase, La2-xSrxNiO4 which has been shown to display colossal dielectric
response due to hopping transport polarization and charge ordering as well as large intercalation of oxygen which leads to interesting growth mechanisms.
1.2 Dielectric Materials
A definitive guide to dielectric phenomena is given in the work by Kao.14 Simply put, a dielectric is an electrical insulator that can be polarized by the application of an electric field. Where the term insulator is used in dc limit for a material with low electrical conductivity, the term dielectric is used almost exclusively in the ac limit, referring to highly polarizable material. One of the most important electrical properties of dielectric materials is the relative permittivity of the material, referred to interchangeable as the dielectric constant. The dielectric constant of a material is the measure of the polarizability of the material with the application of an applied alternating electric field. The polarizability of a material is strongly dependent on the chemical structure and the imperfections (defects) of the material as well as on other physical parameters including temperature, pressure and processing conditions.
Dielectric materials are made up of atoms or molecules that possess one more of the five basic types of electric polarization:
• Electronic polarization • Atomic or ionic polarization • Dipolar polarization
• Spontaneous polarization
• Interface or space charge polarization
Each type of polarization requires a different time scale to perform; this is why the degree of the overall polarization depends on the time variation of the electric field. The time scale is closely dependent on the size of the polarized species. A schematic of the frequency polarization is given in Figure 4 which shows different species polarizing at different frequencies.
Figure 4: General view of the polarization mechanisms as a function of frequency showing approximate mechanism as to where polarization takes place. Reprinted with permission from Ref.. Copyright 2003, American Institute of Physics.
We consider a perfect dielectric material which implies that inside the material no mobile charge carriers (electrons, holes or ions) present. By placing such a dielectric material between two charged plates, the system will tend to attract this piece of material into the vacuum space between the two plates in order to reduce the potential energy of the system. This causes the potential between the plates produced by the original charge to decrease to a smaller value. With the charge on the plates remaining constant, the ratio of the electric field in the space between the charged plates with that of the electric field of the dielectric material. This ratio is the dielectric constant.
A simple parallel plate capacitor, also considered a metal-insulator-metal (MIM), consists of two plates of area A separated by a dielectric material of thickness d. We find that the surface
charge depends on the applied voltage and the quantity measured is the capacitance. In the simple parallel-plate capacitor, the capacitance is given by
C = εrεo where εr is the relative
permittivity of the material (or dielectric constant) and εo is the permittivity of free space. The
voltage and the charge are related by the form Q=CV.
When the relaxation time is much faster than the frequency of the applied electric field, polarization occurs instantly. When the relaxation time is much slower than the frequency of the applied electric field, no polarization (of that mechanism) occurs. When the relaxation time and the frequency of the applied field are similar, a phase lag occurs and energy is absorbed. This is called dielectric loss. It is quantified by the relationship '
'' tan r r ε ε δ = where ' r
ε is the real part of
the dielectric constant and εr''is the imaginary part of the dielectric constant.
There are three major mechanisms of electronic polarization in moderate electric fields (i.e. at fields much lower than the inner atomic or molecular fields) and when the materials has very low conductivity (i.e. the concentration of charge carriers inside the materials is so low that if effects can be negligible). These mechanisms are:
• Electronic polarization: The electric field causes deformation or translation of the originally symmetrical distribution of the electron clouds of atoms or molecules. This is essentially the displacement of the outer electron clouds with respect to the inner positive atomic core.
• Atomic or ionic polarization: Electric field causes the atoms or ions to be displaced relative to each other. This is essentially the distortion of the normal lattice vibration. • Orientation polarization: This polarization occurs in materials consisting of molecules.
Both the electronic polarization and the atomic polarization are due mainly to the elastic displacement of electron clouds and lattice vibration within the atom or molecules. Their interaction is an intramolecular phenomenon, and the restoring force against the displacement is relatively insensitive to temperature so electronic and atomic or ionic polarization processes are only slightly dependent on temperature. Orientation polarization is a rotational process and often times only observed in molecules. Under an external force, it changes to a dynamic equilibrium. When the external field is removed, it relaxes back to its original state.
At higher fields and in “lossy” materials, carrier injection becomes important. For materials consisting of a high concentration of charge carriers (i.e. with a high conductivity), polarization can occur due to the migration of charge carriers to form space charges at interfaces or grain boundaries. This type of polarization is called space charge polarization.
The total polarizability of materials, α, comprises the summation of its polarization mechanismsα =αe +αi +αo +αd where α , e α , i α , o α are the polarizabilities due to d electronic, atomic, orientational and space charge polarizations, respectively. In the following section we will discuss the specific mechanisms dealing with the polarization of ferroelectrics as well as colossal dielectric response materials.
Ferroelectric materials have a permanent electric dipole and due to this, exhibit a spontaneous polarization. Of the 32 point groups, 11 of them are center symmetric which disqualifies them from ferroelectricity. With the application of an external electric field, positive and negative charged atoms will be displaced with respect to the equilibrium position in the unit cell. Of the remaining 21 non-centrosymmetric point groups, they may have one or more polar axes and show piezoelectric effects (except cubic 432). Among the 21 point groups without an
inversion center, there are 10 polar groups which possess a unique polar axis. These crystals may display spontaneous polarization parallel to the polar axis. All ferroelectric crystals belong to a pyroelectric crystal class and have the additional property that an external field can reverse their spontaneous polarization. Thus ferroelectric character cannot be solely determined from crystallography. This reversible polarization manifests itself as a hysteresis loop in the response of polarization to an external applied field.
A ferroelectric crystal shows a reversible spontaneous electric polarization and a hysteresis loop that can be observed in certain temperature regions. For example, in widely studied material, BaTiO3, the perovskite crystal is elongated along the c-axis and the resulting
distortion is termed tetragonal distortion. The body centered Ti atom does not have a preference where to move and creates a built-in polarization along the c axis. With the application of an electric field, the loosely bound Ti will be polarized which brings about the large dielectric constant. Above this temperature region, there is a phase transformation that changes the symmetry of the crystal. In the case of BaTiO3, symmetry is changed to a cubic structure. This
transition point is called the Curie temperature, Tc, and the crystal begins to exhibits paraelectric
dielectric behavior. This occurs since the Ti atom is now energetically favored to sit in the center of the crystal. At T>Tc anomalous behaviors follows the Curie-Weiss relation
C r T T C − = ε
where C is known as the Curie constant. In Figure 5 the Curie temperature (~120°C) of BaTiO3
is shown. As the crystal structure changes with temperature, the dielectric constant (shown along the a-axis and c-axis of the crystal) varies drastically. At 120°C the crystal is cubic and the permittivity along the a-axis and c-axis are equivalent. As the crystal structure changes, there is a change in the dielectric properties of the crystal. More material specific properties of ferroelectrics will be discussed in further in Chapter 184.108.40.206.
Figure 5: Dielectric constant as a function of temperature for a BaTiO3 crystal. Reprinted
from Ref.. Copyright 1949 by the American Physical Society.
1.2.2 Colossal Dielectric Constant Materials
A comprehensive review of the physics behind Colossal Dielectric Constant materials is given by work from the Loidl group.17,18 Most capacitor materials with high dielectric constant are based on ferroelectric which reach values of dielectric constants exceeding 104. However, as mentioned previously, dielectrics exhibit strong temperature dependent dielectric constants, limiting their application into electronic devices. At the moment, the most widely studied non-ferroelectric material exhibiting colossal dielectric response is CaCu3Ti4O12 (CCTO) which was
first reported on 2000.19 The advantage of a material such as CCTO to standard ferroelectric based dielectrics is its nearly temperature independent colossal dielectric response at around room temperature. Only below approximately 200K and as a function of frequency does the
colossal dielectric response show a strong frequency dependence of the magnitude of 100. Typical behavior of colossal dielectric materials is shown in Figure 6.
Figure 6: Behavior of CCTO single crystal showing typical colossal dielectric properties. Reprinted with permission from Ref. . Copyright 2008, American Institute of Physics.
From the first discovery of CCTO, speculations of the colossal dielectric response have been put forward. From the onset, speculations on the origin lay in extrinsic properties of the material namely a barrier layer mechanism. However, certain studies still attributed the response to intrinsic properties of the film. It is commonly accepted that a barrier mechanism is the correct explanation for the response however the nature of these barriers leading to the dielectric response is still open to debate. These include surface barrier layer, internal barrier layer or a combination of the two.
Since CCTO was first discovered to have giant dielectric response, there has been an ongoing search for new and better materials. Many of the isostructural materials have been synthesized in order to discover colossal dielectric response however none have come to give the large dielectric of CCTO.21 Completely different structural transition metal complex oxides have shown interesting dielectric response, namely LSNO, which generate a different mechanism for the large dielectric response.22
Mechanism for Colossal Dielectric Response
To date, the most prominent mechanisms for the colossal dielectric response are as seen in relaxor ferroelectrics,23,24 charge density wave formation,25 hopping charge transport,26 metal insulator transition27 or combinations of the previous effects. For the sake of brevity, we will focus on two of these mechanisms that we observe in this thesis, namely the hopping charge transport and various interface effects leading the increased dielectric response.
Hopping Charge Transport
Hopping conductivity is the most common charge transport process in transition metal oxides. Hopping conduction is the typical charge transport process of localized charge carriers.
In electronic conductors, electrons or holes can be localized due to disorder leading to polaron formation. This disorder may arise from substitutional doping, defects in the lattice or non-stoichiometry.28,29,30,31 Depending on the width and the height of the potential barrier, a charged particle on one site may hop or tunnel to the other site. The hopping conductivity leads to a characteristic frequency dependent power law developed by Jonscher32 and widely referred to as the Universal Dielectric Response. The equation is given as such σ σ υs
where s <1. This response can be understood as the transport of localized charge carriers with such models as variable range hopping. Due to Kramer–Kronig relation, the υs
power law also leads to a corresponding power law in the imaginary part of the ac conductivity, namely
s sπ σ υ σ" 0 ) 2 / tan(
= . Since the dielectric constant is directly related to σ"by
) 2 /(
' σ" πυε0
ε = hopping conduction is expected to lead to a power law of 1
ε . Thus, as s<1, the dielectric constant can reach colossal magnitudes at low frequency. This also leads to tan(sπ /2)on the order of unity. The dielectric loss ε =" σ'/(2πυεo)is extremely high leading many of these systems to be unsuited for device application.33
A detailed study of the interface response is given in Dielectrics and Waves.34 Interfaces of any kind can generate very high apparent values of the dielectric constant because they can act as parallel-plate capacitors with very small plate distances. This effect is known as a Maxwell-Wagner (MW) polarization effect. MW relaxation is a phenomenon having been discussed extensively first by Maxwell and later by Wagner in the 19th century.35,36 Its frequency response spectrum is similar to that of Debye relaxation (dipole relaxation). MW relaxation occur for a variety of heterogeneities, including a depletion layer between a sample and electrode, interfacial
layer of grain boundaries and electronic heterogeneities which may occur from charge ordering. Domain boundaries are also suggested as another source at which M-W relaxation can occur.37
The heterogeneity associated with different contacts (electrodes, interfaces, and grain boundaries) can be modeled by a two layer model shown in Figure 7 which consists of two RC
(R=resistance and C=capacitor) circuits in series, one for the contact and the other for the
sample. The dielectric properties of the system can be characterized by the conductivities σ i
(i=1,2) permittivities εi and thickness di with the real and imaginary parts of the complex
permittivity can be written as38,39
ω σ ε ε ε ε ε* = '−j ''= r o − j where 2 ' ) ( 1 ) ( ωτ ε ε ε ω ε + − + = ∞ ∞ s 0 2 ) ( 1 ) ( ) ( " ωε σ ωτ ωτ ε ε ω ε + + − = s ∞
From Figure 7, the static limit, εsand the high frequency limit, ε∞ are given by
1 1 ) 0 ( ' d d s ε ω ε ε = = = ) ( ) ( ' 2 1 1 2 2 1 ε ε ε ε ω ε ε d d d + = ∞ → = ∞
By extending this analysis of the two layer system in the terms of conductivity, it can be shown that the dielectric dispersion of a two layer system can be described to be Debye-like but the high frequency and low frequency terms can be described in terms of the two materials sharing an interface
17 2 2 1 1 2 2 1 2 2 2 2 1 1 ) ( ) ( ) 0 ( ' σ σ σ ε σ ε ω ε ε d d d d d s + + = = = ) ( ) ( ' 2 1 2 1 2 1 ε ε ε ε ω ε ε d d d + = ∞ → = ∞
where the relaxation time for the interfacial polarization is given as
1 2 2 1 2 2 1 1 d d d d σ σ ε ε τ + + =
where d=d1+d2, ω and ε0 is the thickness of the entire layer, the angular frequency and the
permittivity of free space, respectively.
The relaxation time and therefore the dispersion frequency are related to the permittivity and conductivity values of both materials. The cause for the effect can be explained as follows: The dielectric material between the two plates has a net total impedance and therefore must give a constant current through the structure. Since the two materials transfer charge in different ways (by conduction or polarization), there exists a discontinuity at the interface between the materials where the mode of charge transfer changes. Where one transfers charge principally by conduction and the other by polarization, an accumulation of charge at the interface occurs. Therefore, a dipole is created at the interface. Interfaces in a material, i.e. electrical inheterogeneities, grain boundaries, etc. lead to a significant interfacial effects.
Figure 7: Maxwell-Wagner two layer capacitor model. Adapted from Dielectrics and Waves (Ref.).
Of significant interest to this dissertation is the spontaneously arising interfaces caused by electronic phase separating arising from charge ordering in certain transition metal complex oxides. This phenomena has been seen in systems exhibiting high Tc superconductivity
(La2CuO4), magnetoresistance manganites and nickelates.40 The system La2-xSrxNiO4 has
attracted significant interest due to stripe like and checkerboard ordering in much of its phase diagram.41 Due to the process of charge ordering, internal interfaces develop leading to the enhanced observed polarization. This leads to a Maxwell-Wagner type response and can be regarded as quasi-intrinsic. These interfaces may lead to delayed dispersion due to the fine length scale or can be coupled with other mechanisms to give a higher apparent polarization.
1.3 Motivation of Thesis
1.3.1 Bypass Capacitors for Next Generation System on
Tremendous progress has been made in the past four decades in miniaturizing and integrating transistors and capacitors for logic applications onto silicon in keeping with the semiconductor industry’s decades-old defining paradigm of Moore’s Law. By comparison, passive components (resistors, capacitors and inductors) on the circuit-board level have made only incremental advances in size and density, sometimes referred to as the system integration law and shown in Figure 8.42
Passive components refer to non-active elements, including capacitors, resistors and inductors and usually tens to hundreds of discrete passive components are mounted on the circuit board. Consequently, passive components occupy an increasingly larger area and mass fraction of electronic systems and are a major hurdle to the miniaturization of many electronic systems.
Figure 8: Moore's Law and System Integration Law. Reprinted with permission from Ref. . Copyright 2006, IEEE.
Embedded passive components could be defined as passive components sandwiched between the interconnecting layers of a circuit board, including printed wiring board and ceramic tape. The goal of embedded passive components is to take surface mount technology (SMT) from top and/or bottom of the board and to bury those components in the board thickness as seen in the evolution and predictions in Figure 9. By moving from SMT to embedded passives, significant improvement in performance and size can be obtained. Reduced system mass, volume and footprint with the integration of the package into the substrate leaves more room on the surface for the ICs. Improved electrical performance is achieved due to lower parasitics,
particularly lower inductance due to shorter signal transmission as well as minimizing loop inductance.43 Embedded passives may also improve reliability by the elimination of solder joints. The eventual goal is to achieve what is known System on Package (SoP) technology which allows for all passives to be integrated along with some active components into the packaging board. A look at the future concept is seen in Figure 10. This is reviewed in detail by in Fundamentals of Microsystems Packaging.44
Figure 9: Projected evolution from Surface Mount Technology (SMT) to Embedded Passives. Reprinted with permission from Ref..
Figure 10: Future view of a System-on-Package. Note the placement of the decoupling capacitor. Reprinted with permission from Ref.. Copyright 2006, IEEE.
In order to reach this goal, thin film capacitors (decoupling or bypass capacitors) on non-noble metallic foils need to be developed to replace the existing bulk ceramic surface mounts. These thin film capacitors could be embedded directly beneath the IC rather than spread out across the printed wiring boar. Thus would decrease the amount of area the wiring board requires and improve speed and performance directly related to the distance between the capacitor and the IC.
In order to achieve these goals, key technical issues must be surmounted. The growth of high quality dielectric materials with dielectric density on the order of 10-100 μF/cm2 would be needed as well as the growth of these materials at low enough temperatures to allow for the incorporation with existing dielectric circuit boards and IC components. These materials (preferably non-noble to reduce cost) should be readily incorporated into the supply chain. To date, thin film capacitor technology has not yet been developed that would satisfactorily replace current bulk ceramic capacitors of all capacitance values used in modern electronic packages.
The challenge here is to identify a material suitable for dielectric processing where thin film properties of this material can be compatible with the semiconductor industry roadmap. This requires us to identify materials that should be researched to try to achieve these targets.
1.3.2 Material Studied
In this thesis, the properties of two complex oxides in thin film form will be discussed: Ba1-xSrxTiO3 and La2-xSrxNiO4. The first part of the thesis delves into the solid solution of
BaTiO3 and SrTiO3 with the chemical structure Ba1-xSrxTiO3 (BST) which displays large
paraelectric polarization. With this material we investigate the effect of oxygen stoichiometry on the dielectric properties and investigate novel processing methods for growth on non-noble electrodes.
The second material studied is the Ruddlesden-Popper phase, La2-xSrxNiO4, which has been
shown to display colossal dielectric response as well as large intercalation of oxygen which leads to interesting growth mechanisms.
Barium Strontium Titanate (BST), BaxSr1-xTiO3, where 0≤ x≤1 is a solid solution of
BaTiO3 and SrTiO3. BST has a perovskite crystal structure with the formula ABO3. In BST, the
A site is occupied by Ba and St (oxidation state of +2) atoms while B site is occupied by Ti (oxidation state of +4) while O ion is in the -2 oxidation state. Ba2+ and Sr2+ are located in the eight corners of the cubic crystal cell and O2- is located at the face of the cube while the Ti4+is located at the center of the cubic cell.
BaTiO3 as discussed earlier is a ferroelectric at room temperature (Tc = 120C) while
of Ba:Sr as seen in Figure 11 and Figure 12. Electrical properties are also greatly dependent on the stoichiometry of the material, in particular the cation ratio and oxygen concentration. An important application based property of BST is the ability to change the dielectric constant and dielectric loss tangent near the Curie temperature by an externally applied field, which makes this material ideally suited for electrically tunable devices such as phase shifters and filters. This is due to the paraelectric phase having a centrosymetric tunability.46,47
Figure 11: Effect of cation ratio on the crystal structure of BST. Reprinted with permission from Ref. . Copyright 1997, American Institute of Physics.
Figure 12: Effect of cation ratio on the Curie temperature of BST. Reprinted with permission from Ref.. Copyright 1997, American Institute of Physics.
Besides the concern for the cation ratio, great emphasis is placed on the oxygen stoichiometry. Due to charge balance, oxygen vacancies lead to n-type conductivity by the
equation, ( ) 2 1 ' 2e O2 g V
OOx = O••+ + . Kroger-Vink notation is used where x O
O is the Oxygen on the oxygen site with a neutral charge, ''
V is the vacancy on the oxygen site with a net positive charge, and two electrons with a negative charge each to balance the equation. Oxygen vacancy therefore gives the lattice more n-type carriers and greatly increases the leakage in the material. In order to consider device application, where a robust low loss dielectric must be used, maintaining stoichiometry is of great concern. Measuring the electronic conductivity as a function of low partial pressure has shown a dramatic dependence on the partial pressure and therefore oxygen content of the material as seen in Figure 13. The slope of the graph, showing a
-1/4 dependence indicates an n-type conductivity at low partial pressures and a p-type conductivity at high partial pressures. When depositing thin film material or growing bulk samples of BST, the crystal may become oxygen deficient. This also occurs with the deposition of electrodes due the process of impinging the metal material onto the surface. In order to make high quality material, ways to reintroduced lost oxygen must be developed.
Figure 13: Electrical conductivity in polycrystalline BaTiO3 as a function of partial
pressure. Reprinted with permission from Ref.. Copyright 1985, Annual Reviews.
Since the discovery of high Tc superconductivity by Bednorz and Muller in 1986, there
has been a deep interest into the La2-xBaxCuO4 structure as well as isostructural materials in